Search the Community
Showing results for tags 'paper developer'.
Found 1 result
Hello guys and gals, So, yesterday, while processing some Tri-X Super 8, something nightmareish happened during the second developpement after re-exposure : after 1 min in the 2nd developer (where the emulsion properly reacted and darkened), it slightly started to lift from the plastic and then it litteraly disloved into the developper : no floating gelatin flakes, just a plain black developer... The weird thing is that I already processed Tri-X this way, here is an example : https://vimeo.com/326184819 Here is my protocole, I have included as much info as I can : 1 – Soaking in a 25°C water bath. 2 – 1st Developer : Ilford Multigrad 1+9, 20min (continuous agitation on 1st minute, then 10sec each minute), 25°C. 3 – Hardening stop bath : Adox EcoStop 1+29 + 40ml/L of Tetenal Hardener. 6 min, 20°C, continuous agitation. (https://www.fotoimpex.com/chemistry/tetenal-hardener-to-be-added-to-the-fixer-or-stop-bath-1000-ml.html?cache=1564733928) 4 – Washing, runing water, 2 minutes. 5 – Bleach : Potassium permanganate 0,4% + Sulfuric Acid 10% equal part, 6 min, 20°C, continuous agitation. 6 – Washing, runing water, 2 minutes. 7 – Clearing bath, Sodium metabisulfite 6%, 2 min, 20°C, continous agitation. 8 – Washing, runing water, 2 minutes. 9 – Hardening stop bath : Adox EcoStop 1+29 + 40ml/L of Tetenal Hardener. 6 min, 20°C, continuous agitation. 10 – Washing, runing water, 2 minutes. RE-EXPOSURE : 2x1min 80W 1m in a white tank filled with water. 11 – 2nd Developer : Ilford Multigrad 1+9, 4min (stand), 25°C. The same solution I used as 1st developer. And that's where the emulsion dissolved.... Usually, after that, I use an hardening fixer for 5 minute, washing 10 min on runing water, rinse with distilled water, let it dry and digitalise with a Retroscann Universal. It's fastidious, but cheap ! Side notes : - Processing in Lomo Tank. - I know Ilford says not to use Ilford Multigrade for processing film (Universal PQ is recommanded instead), but through my test phase it was the only thing I had on hand, so I tried and it worked as you could see on vimeo. - I've never found any information about the shelf lif of the Tetenal hardener. As it is supposed to be mixed with Stop or Fix, I mixed it with the Adox Eco Stop to be sure I won't use an hardening bath tha is no longer working. Anyway, I mixed a new solution and it was still a disaster. - I use the hardener to compensate the softening of the emusion by the bleach. One bath before to strenghten, one bath after to reinforce. I thing the bleach isnt to blame, otherwise it the continous agitation in the clearing bath would have the same mechanical effect, so I guess it is a chemistery issue. The film is perfectly fine during re-exposure, bleaching is complete, after touching the film, the emulsion is normal. - I dont know why the developper is dissolving the emulsion on second use but work perfectly fine on the first one. So that's it, if anyone have an idea, i'm all ears ! Thanks ! Jérémy